Journal of Alloys and Compounds 618 (2015) 64–66
Contents lists available at ScienceDirect
Journal of Alloys and Compounds journal homepage: www.elsevier.com/locate/jalcom
CaO dissolution during melting and solidiﬁcation of a Mg–10 wt.% CaO alloy detected with in situ synchrotron radiation diffraction B. Wiese a,⇑, C.L. Mendis a, D. Tolnai a, A. Stark b, N. Schell b, H.-P. Reichel c, R. Brückner c, K.U. Kainer a, N. Hort a a b c
MagIC – Magnesium Innovation Centre, Helmholtz-Zentrum Geesthacht, Max-Planck-Straße 1, D-21502 Geesthacht, Germany Materials Physics, Helmholtz-Zentrum Geesthacht, Max-Planck-Straße 1, D-21502 Geesthacht, Germany LMpv Leichtmetall – Produktion & Verarbeitung GmbH, Einsteinstraße 4, D-36466 Dermbach, Germany
a r t i c l e
i n f o
Article history: Received 18 June 2014 Received in revised form 15 August 2014 Accepted 18 August 2014 Available online 27 August 2014 Keywords: Magnesium alloys Solidiﬁcation Liquid–solid reactions Synchrotron radiation In situ phase evolution
a b s t r a c t The phase dissolution and evolution during the melting and the solidiﬁcation of Mg containing 10 wt.% CaO was investigated in the temperature range of 20–680 °C. The dissolution of CaO and the formation of Mg2Ca were detected with in situ synchrotron radiation diffraction. The dissolution of CaO was observed at 407 °C with the detection of a peak unique to the Mg2Ca phase prior to melting of Mg. After the solidiﬁcation no CaO was detected, and Mg2Ca and MgO phases were observed. Ó 2014 Elsevier B.V. All rights reserved.
1. Introduction The interactions between Mg and CaO affect the evolution of the microstructure, the mechanical and the corrosion properties of the newly developed ECO (Environment COnscious) Mg alloys . Previous investigations on CaO addition to pure Mg [1–4] and Mg alloys [1,3,5–7] report that the CaO disperses in Mg. These investigations were made on as-cast samples [1–3,6,7] and samples processed via Equal Channel Angular Bulk Mechanical Alloying (ECABMA) subsequently heat treated . After solidiﬁcation or heat treatment, previous investigation reported, the formation of Laves phase Mg2Ca in pure Mg and Al2Ca in Mg–Al alloys. According to the Ellingham diagram CaO is more stable than MgO , therefore, it is expected that CaO remains unreacted. Kondoh et al.  calculated the standard Gibbs free energy for the reaction between pure Mg and CaO using Eq. (1). This thermodynamic hypothesis showed a decrease in the standard Gibbs free energy for the disassociation of CaO and the formation of Mg2Ca Laves phase at low temperatures . Kondoh et al.  investigated the solid state reaction between CaO and AZ61 which forms Al2Ca after mechanical alloying. It is necessary to understand the reactions between Mg and CaO in the solid and liquid states to elucidate ⇑ Corresponding author. Tel.: +49 4152 871963; fax: +49 4152 871909. E-mail address: [email protected]
(B. Wiese). http://dx.doi.org/10.1016/j.jallcom.2014.08.151 0925-8388/Ó 2014 Elsevier B.V. All rights reserved.
the thermodynamics behind the dissolution of CaO. Therefore, it is important to determine which phases are present during heating, in the melt, during solidiﬁcation; and to follow the dissolution of CaO in pure Mg. This contribution reports the ﬁrst in situ investigation on the dissolution of CaO in Mg during melting and solidiﬁcation.
3Mg þ CaO ! Mg2 Ca þ MgO
2. Material and methods In the present study, the melting- and the solidiﬁcation behaviour of pure Mg (chips produced by cutting with a machine) mixed with 10 wt.% CaO powder was investigated in the temperature range from room temperature to 680 °C using synchrotron radiation. The 10 wt.% CaO was chosen to identify the dissolution of CaO in Mg and to ensure the volume fraction of pertinent phases remain above the measurement threshold. This allows the detection of the various reactions that occur during in the heating, holding and cooling. The synchrotron radiation diffraction study was conducted at the P07 (High Energy Materials Science) beamline of PETRA III (Deutsches Elektronen-Synchotron), with a beam energy of 100 keV (k = 0.0124 nm) and a beam cross section of 1 1 mm2. The samples were heated with the induction coil of a Bähr 805A/D dilatometer modiﬁed to prevent interaction of the coil with the X-ray beam. The set-up is isolated with two windows covered with Kapton foils so that the X-ray beam interacts only with the sample [9,10]. The samples were heated in an Ar atmosphere to 500 °C at 100 K min1, then to 680 °C at 10 K min1. The samples were held at 680 °C for 5 min to ensure melt homogeneity, and then cooled at 10 K min1 to 500 °C (fully solidiﬁed state) before air-cooling to room temperature. The temperature–time–curve was controlled by a
B. Wiese et al. / Journal of Alloys and Compounds 618 (2015) 64–66
S type thermocouple welded on the stainless steel crucible (ME-00029990 120 ll from METTLER-TOLEDO made from stainless steel with a wall thickness of 0.33 mm) containing the pure Mg and CaO powder sample. The two dimensional (2D) diffraction patterns were recorded in transmission geometry at every 6 s with an acquisition time of 3 s with a PerkinElmer XRD 1622 Flatpanel at a sample-todetector-distance of 1452 mm. This results in a resolution of 10 K for heating at 100 K/min and a resolution of 1 K during heating and cooling at 10 K/min. Consequently the temperature resolution for the heating at 100 K/min is ±10 and heating or cooling at 10 K/min is ± 1. X-ray line proﬁles were obtained by azimuthal integration of the 2D diffraction patterns through 360°. For phase identiﬁcation simulated line proﬁles were generated with CaRIne 3.1 Crystallography™ with crystal structure data from the Pearsons Crystallography Database . Separate samples for bulk investigations, including scanning electron microscopy (SEM), are produced by casting from pure Mg ingots (99 g) with 10 wt.% CaO (11 g) in a steel crucible using electric furnace (Hornbach Spezialmaschinen GmbH). The melt was held at 680 °C and mixed with CaO powder and held steering for 5 min, and then cast into steel mould (Ø18x180 mm) preheated to 350 °C. The specimens for SEM were prepared by grinding with SiC paper to 2500 grit, polishing with a 3 lm diamond suspension followed by a mixture of 1 lm diamond and OPS™ anhydrous suspension. Microstructures were investigated using a Carl ZEISS, ULTRAT M 55 SEM, operating at 15 kV, equipped with an EDAX energy-dispersive X-ray spectrometer (EDXS) and the local compositions determined by point analysis and compositional maps.
3. Results and discussion The SEM investigation of the as-cast Mg–10 wt.% CaO sample shows the formation of the Mg/Mg2Ca Laves phase lamellae eutectic in the a-Mg matrix shown in Fig. 1. As cast bulk samples were used for the SEM investigation as the sample used for the in situ synchrotron study could not itself be used for this investigation. The EDXS point analysis (arrowed in Fig. 1a) in this eutectic region shows a Ca content of 8 at.%. The EDX maps of Ca and O show that there is no O enrichment associated with Ca (Fig. 1b and c). However, with EDXS point analysis (Fig. 1d) a small O peak is detected (1.3 at.%). The O content is signiﬁcantly lower than Ca, thus this phase is unlikely to be pure CaO. Due to the low solid solubility of Ca in Mg (1.34 wt.%/0.8 at.%) any segregation of Ca that occur within a-Mg grains during solidiﬁcation cannot be observed on the EDXS elemental map for Ca. The X-ray line proﬁles from the synchrotron investigation show the dissolution of CaO and the formation of Mg2Ca and MgO phases during the heating and cooling cycle of the experiment (Fig. 2a). In the powder state the peaks from CaO and Mg are observed. During heating the Mg peaks shifts to smaller angles, as the thermal
Fig. 2. Selected line proﬁles (a) up to the melting stage and (b) isothermal holding and solidiﬁcation with the observed phases indicated.
expansion results in a slight increase in the lattice parameters. The line proﬁle at 407 ± 10 °C shows a double peak at 2.7° that is comprised of diffraction due to Mg and Mg2Ca, as illustrated by the line at 500 °C, Fig. 2a. In the molten state (at 642 ± 1 °C) the intensity of the CaO peaks decrease rapidly while the MgO peak
Fig. 1. (a) Scanning electron micrograph (SEM) of as-cast Mg–10 wt.% CaO alloy. EDXS map of the same area showing (b) Ca and (c) O. (d) EDX spectra recorded from the area as indicated by the arrow.
B. Wiese et al. / Journal of Alloys and Compounds 618 (2015) 64–66
of the CaO (2 0 0) peak observed at 600 °C. It is proposed that in this temperature a reaction layer forms around CaO particles and a critical layer thickness, with high concentration of Mg2Ca/MgO. Since this layer can act as a diffusion barrier as it slows down the dissolution of the CaO in Mg. The ﬁrst set of unique Mg2Ca peaks appear during solidiﬁcation at 505 ± 1 °C, which is below the eutectic temperature of the Mg rich side of the Mg–Ca phase system, 516 °C. The presence of O leads to the ternary phase system Mg–Ca–O which can reduce the eutectic temperature for Mg2Ca formation. It is possible that this can explain the reduction of the eutectic temperature for the formation of the Laves phase Mg2Ca. However, there is no sufﬁcient information on the Mg–Ca–O system available to conclusively determine this. Another possibility could be the reaction kinetic of the phase formation in the cooling process. During further heating more Mg2Ca forms. However, the Mg2Ca phase dissolves in liquid Mg above 650 °C as the total content of Ca (3 wt.%) in the alloy is less than the Ca content required for Mg2Ca to remain stable above 650 °C. The formation of Mg2Ca Laves phase following solidiﬁcation is consistent with the previous investigations [2,3,7]. 4. Conclusions
Fig. 3. The disassociation of CaO in the Mg (a) peak evolution with the intensity change for (2 0 0) CaO peak and (b) change in the integrated intensity of (2 0 0) CaO peak relative to (2 0 0) CaO peak at 600 °C.
intensity increased. The CaO peaks (2.6° and 2.9° in 2h) disappear after holding for 5 min at 680 °C but the overlap peaks for Mg2Ca and CaO (4.14° and 4.91° in 2h) remained due to the formation of Mg2Ca. To understanding the dissolution of CaO we used the (2 0 0) peak from CaO as this peak does not overlap with another phase that were expected in the system (i.e. Mg, MgO or Mg2Ca phases). We have not conducted a systematic Rietveld analysis to determine the phase fraction as the investigated sample is not an ideal powder sample. This is related to the slower cooling rate and the grain growth that lead to a non-random distribution of grain orientations. Fig. 3a shows the main CaO peak (2 0 0) and the method used to integrate the peak area. Only the area under the curve without background was used as the integrated peak area. The peak evolution in Fig. 3b shows the change of the integrated peak area of CaO (2 0 0) peak during heating, and the dissolution of CaO in the solid and molten Mg is illustrated. In order to follow the dissolution of CaO easily the integrated peak area of CaO (2 0 0) peak was normalised to the CaO (2 0 0) peak at 600 °C. The dissolution of CaO starts below the melting temperature of Mg as indicated by the presence of Mg2Ca. The reduction of CaO to Ca starts during heating in solid-state before Mg melts. From 600 °C to the melting temperature of Mg (650 °C) the dissolution speed increases, and is expected to be proportional to the solid-state diffusion co-efﬁcient of Ca in Mg. In the molten state (above 650 °C) the dissolution speed of CaO increased signiﬁcantly, as the diffusion in the liquid Mg is higher than that in the solid Mg. During holding at 680 °C the change in the integrated peak area (dissolution speed) decreases and become constant as shown in Fig. 3b. After cooling to 600 °C the CaO (2 0 0) peak decreased to 0.007 that
The investigation on the Mg–10 wt.% CaO system followed the phases evolution during heating, in the molten state and during solidiﬁcation. The dissolution of CaO in Mg was not expected from Ellingham diagram, but the measurement show the ﬁrst interaction between Mg and CaO and formation of Mg2Ca occurs at 407 ± 1 °C. The dissolution speed increased with the temperature and the dissolution speed signiﬁcantly increased between 600 °C and 640 °C in the pre-molten state. The reaction in the pre-molten state between Mg and CaO was detected for the ﬁrst time during an in situ investigation. This type of investigation open the possibility to understand the role of CaO in Mg and Mg based alloys. This information can be used for evaluation of thermodynamic calculations and experimental veriﬁcation of phase diagrams of Mg alloys contenting CaO. Acknowledgements The authors acknowledge the Deutsches Elektronen-Synchrotron for the provision of synchrotron radiation facilities within the framework of the proposal I-20120285 and the Federal Ministry for Economic Affairs and Energy (BMWi) funding for the project MagHyM (20K1107B). References  Shae K. Kim, in: Frank Czerwinski (Ed.), Design and Development of HighPerformance Eco-Mg Alloys, Magnesium Alloys – Design, Processing and Properties, InTech, , 2011, ISBN: 978-953-307-520-4, DOI: 10.5772/13836.  S.-H. Ha, J.-K. Lee, H.-H. Jo, S.-B. Jung, S.K. Kim, Rare Metals 25 (2006) 150–154.  S.-H. Ha, J.-K. Lee, S.K. Kim, Mater. T. JIM 49 (2008) 1081–1083.  Y.-B. Huang, I.-S. Chung, B.-S. You, W.-W. Park, B.-H. Cho, Met. Mater. Int. 10 (2004) 7–11.  K. Kondoh, J. Fujita, J. Umeda, H. Imai, K. Enami, M. Ohara, T. Igarashi, Mater. Chem. Phys. 129 (2011) 631–640.  N.D. Nam, M.Z. Bian, M. Forsyth, M. Seter, M. Tan, K.S. Shin, Corros. Sci. 64 (2012) 263–271.  J.-K. Lee, S.K. Kim, Mater. T. JIM 52 (2011) 1483–1488.  I. Brain, O. Knacke, Thermochemical Properties of Inorganic Substances, Springer-Verlag, Berlin, New York, 1973.  P. Staron, T. Fischer, T. Lippmann, A. Stark, S. Daneshpour, D. Schnubel, E. Uhlmann, R. Gerstenberger, B. Camin, W. Reimers, E. Eidenberger, H. Clemens, N. Huber, A. Schreyer, Adv. Eng. Mater. 13 (2011) 658–663.  D. Tolnai, C.L. Mendis, A. Stark, G. Szakács, B. Wiese, K.U. Kainer, N. Hort, Mater. Lett. 102–103 (2013) 62–64.  P. Villars, K. Cenzual, Pearson’s Crystal Data – Crystal Structure Database for Inorganic Compounds (on CD-ROM), Materials Park, Ohio, USA, 2012.